**Theoretical Study of the Rare Earth Compounds **

**LaFe**

**13-x**

**13-x**

**T**

**x **

**x**

**(T = Cr, Cu, Ga, Mn, Ni) and Curie **

**Temperature Variation **

**Lingping Xiao****1,2*****, Jiang Shen2**

1_{Jiangxi Blue Sky University, Nanchang, China; }2_{Institute of Applied Physics, University of Science and Technology, Beijing, China.}

Email: *****_{xiaolingping1982@163.com }

Received November 25th_{, 2010; revised January 17}th_{, 2011; accepted June 9}th_{, 2011. }

**ABSTRACT **

*The phase stability and site preference of the intermetallics LaFe*13*-xTx (T = Cr, Cu, Ga, Mn, Ni) with NaZn*13*-type *
*struc-ture have been investigated by lattice inversion potentials. The calculated results indicate that each of the stabilizing *
*elements Cr and Mn significantly decreases the cohesive energy of LaFe*13-*xTx and plays a role in stabilizing the 1:13 *

*structure. The calculated lattice parameters of LaFe*13-*xTx (T = Al, Si) compounds are in good agreement with the *

*ex-perimental data. Qualitative analyses are carried out on the behavior of the Curie temperature and magnetocrystalline *
*anisotropy. All the results indicate that the pair potentials based on the lattice inversion method can effectively give a *
*deeper insight into the structure and property of complex materials. *

* Keywords*:

*Rare Earth Compounds, Interatomic Potentials, Site Preference, Computers Simulation*

**1. Introduction **

Recently rare earth transition metal intermetallic
com-pounds with NaZn13-type structure have attracted
con-siderable attention owing to their potential application
and intriguing magnetic properties [1-4]. In rare earth-
transition metal intermetallic compounds the strong
magnetic coupling between 3d atoms gives rise to the
large magnetization. It seems that the novel R-T
inter-metallic compounds with excellent magnetic properties
are always related to a high content of 3d transition metal.
Among all binary R-M intermetallic compounds only
LaCo13 crystallizes in the cubic NaZn13-type structure
(space group Fm-3c). The LaFe13 compound does not
exist. Generally, the positive heat of alloying between La
and Fe is considered to be the reason why no LaFe13
bi-nary compound exists. Up to now, many compounds
with NaZn13-type structure have been obtained in R (T,
M) 13 systems (R = rare earth, T = Fe, Co, Ni and M = Al,
Si) by elemental substitution. By now ternary compounds
LaFe13-*x*Si*x* (1.3 < x < 2.6) [5] and LaFe13-*x*Alx (1 < x < 7)
[6] are known. Besides, recently the NdFe13-*x*Be*x*

com-pounds (2< x <4) have been synthesized.

The cubic symmetry of the structure usually implies a lack of significant magnetocrystalline anisotropy, so that intermetallic compounds with the NaZn13-type structure

cannot be used for permanent magnets. Much larger
magnetocrystalline anisotropy is expected in materials
with a strong anisotropic crystal structure. It has been
observed that in some range of Si or Al concentrations
the crystal symmetry of the R(M,T)13 compounds
trans-forms from cubic (NaZn13-type) to tetragonal in the
LaCo13-*x*Si*x* and PrFe13-*x*Si*x* compounds (Ce2Ni17Si9-type)
[7] or to orthorhombic in the LaFe13-*x*Al*x* compounds[8]

and hence creates an opportunity for developing magne-tocrystalline anisotropy in 1:13 alloys.

In this work, a series of inter-atomic pair potentials in
LaFe13-*x*T*x* were determined using a general lattice-inversi-

on technique with a first principles-based crystal
cohe-sive energy calculation. In this way, the stability of
LaFe13-*x*T*x* and the site preference were evaluated and

analyzed. Section 2 given an introduction to the method-ology for the calculation. Section 3 shows the calculated results and give a comparison with the results of the ex-periments. The conclusions and the further discussion are given in the Section 4.

**2. Calculation Methods **

principle calculation or by experimental data fitting. The lattice inversion theorem is focused on explaining how to use Chen’s lattice inversion theorem to obtain the intera-tomic pair potential from the first principle cohesive en-ergy curve. A brief introduction of the lattice inversion theorem is proposed as follows [9]: Suppose that the crystal cohesive energy obtained by the first principle calculation is expressed as:

E(x) = 0 0

1

1 _{[ ( ) ]}

2*n*

*r* *b n x*

###

(1)where *x *is the near-neighbor distance, r0(n) is the n
neighbor coordination number, b0(n)x is the distance
be-tween the central reference atom and its nth neighbor,
and [b0(n)x] is the pair potential. A multiplicative
closed semi-group b(n). In the process, a lot of virtual
lattice points are involved, but the corresponding virtual
coordination number is zero. In the b(n), for any two
integers m and n, there is a sole integer k such that b(k) =
*b(m) b(n). Hence, equation (1) can be rewritten as *

###

E(x) = _{0}

1

1 _{[ ( ) ]}

2*n*

*r b n x*

###

(2)where

###

###

###

1###

0 ( )

( ) _{0}*r b* *b n n*

*r n*

###

(3)###

0###

0

( ) ( )

( ) ( )

*b n* *b n*

*b n* *b n*

###

Then the general equation for the interatomic pair po-tential obtained from the inversion can be expressed as

( ) 2 ( ) [ ( ) ]

*n i*

*x* *I n E b n x*

###

(4)where I(n) has the characteristics of

1

1 ( )/ ( )

( ) ( )

( ) *k*

*b n b k*

*b k*
*I n r b*

*b n*

###

(5)*I(n) is uniquely determined by a geometrical crystal *
structure, not related to the concrete element category.
Thus, the interatomic pair potentials can be obtained
from the known cohesive energy function E(x).The
in-teratomic pair potential in distinct atoms can be obtained
by the same inversion method, and they are used to study
the rare earth intermetallics structures. Which are close to
the Morse function, that is:

###

01 2

0

x = 2

*x* *x*

*R* *R*

*Ф* *D e* *e*

_{} _{} _{}_{} _{} _{} _{}_{}
_{}
0
1
_{}

(6)

where *D*0 is the depth of potential of potential, R0, *γ* are
parameters. Some important potential are show in the

**Table 1. **

**3. Calculation Results **

The structure of LaFe13-*x*T*x*(T = Ga, Ni, Mn, Cr, Cu)

compounds are simulated by the energy minimization process and realized by the conjugate gradient method with 14 Å as the cut-off radius of the potentials. The re-sults are taken by the arithmetic average for 30 stochastic configurations. To avoid statistic fluctuation, the model is taken as a 2 × 2 × 2 super cell.

**3.1. Phase Stability and Lattice Constants of **
**LaFe****13-x****T****x ****(T = Cr, Cu, Ga, Mn, Ni) **

Although the pure LaFe13 compound is unstable, it can be
considered as the eigentructure of LaFe13-*x*T*x* and their

interstitial compounds. In the calculation procedure, the initial lattice constants of LaFe13 are randomly chosen in a certain range. Under the control of the interatomic pair potentials, the energy minimization is carried out by us-ing the conjugate gradient method. The results show that the space group maintains Fm-3c or I4/m·cm with NaZn13-type structure in the tolerance range of 0.001 - 0.1 Å.

In the structure of LaFe13, we first substitute T (T = Cr,
Cu, Ga, Mn, Ni) atom for Fe in each site with different
concentrations and then use the energy minimization
method to relax the systems under the interaction of the
potentials. With different fractions of the third element,
LaFe13-*x*T*x* may crystallize in the cubic structure with the

space group Fm-3c or in the tetragonal structure with the
space group I4/mcm. Thus the average cohesive energy
of final structure can be investigated and compared. The
average cohesive energies of different structures are
displayed in **Figure 1**. It can be seen that the crystal

energy gradually decrease with increasing content of the ternary element T (T = Cr, Cu, Ga, Mn, Ni). The struc-ture stability is judged by the energy and tolerance. The tolerance, which represents the displacement of the atomic position in order to retrieve the space group, is an assistant criterion. Numerous calculations show that, when the tolerance is much large than 0.5 Å，the com-pounds do not exist in experiments. In fact, the site oc-cupation is determined by the energy and the too large tolerance means that the final stable structure has devi-ated too far from the selected one and that the structure has been changed.

In the calculation, for LaFe13-*x*Cr*x*, Cr entering into 96i

structure is acceptable for x ≤ 3.75. For LaFe13-*x*Mn*x*, Mn

entering into 8b site of the cubic structure has the lowest energy for x ≤ 3.25, and the tolerance is acceptable in this range. However, in the range of 3.25 ≤ x ≤ 4.0 the toler-ance with Mn entering into 96i site of the cubic structure

is so large that the cubic structure could not exist, and
Mn entering into 16k site of the tetragonal structure.
From the **Figure 1**, we can see that Cr, Mn play an

im-portant role in stabilization. But Ni, Cu and Ga cannot stabilize LaFe13 structure.

**Table 1. Some important potential of (LaFe13-xTx) system. **

*R*0(Å) *D*0(kcal/mol) *γ*

Fe-Fe 2.73609 17.6177 8.75429 La-La 4.7585 6.7761 6.4607 La-Fe 2.41269 2.38229 6.30159

La-Si 3.4186 13.2643 10.0062

La-Al 3.64488 10.6466 8.89225 Fe-Si 2.7334 15.2938 8.2601

Fe-Al 2.7405 14.9015 9.09675

0 1 2 3 4 5 6

-6.25 -6.20 -6.15 -6.10 -6.05 -6.00 -5.95 -5.90

-5.85 (LaFe13-xCrx)

Cohes

iv

e Energy

(ev

/at

om)

Cr content (x)

8b 4d 96i 16k 16k(1) 16k(2)

0 1 2 3 4 5 6

-0.1 0.0 0.1 0.2 0.3 0.4 0.5 0.6 0.7 0.8

(LaFe_{13-x}Cr_{x})

to

er

la

nc

e

Cr content (x)

0 1 2 3 4 5 6 -5.8

-5.6 -5.4 -5.2 -5.0 -4.8 -4.6 -4.4

(LaFe_{13-x}Cu_{x})

C

ohesive E

n

ergy

(e

v/

a

tom)

Cu content (x)

8b 4d 96i 16k 16k(1) 16k(2)

0 1 2 3 4 5 6

-0.1 0.0 0.1 0.2 0.3 0.4 0.5 0.6 0.7 0.8

0.9 (LaFe13-xCux)

to

le

ra

n

c

e

Cu content (x)

8b 4d 96i 16k 16k(1) 16k(2)

0 1 2 3 4 5 6

-6.0 -5.8 -5.6 -5.4 -5.2 -5.0 -4.8 -4.6 -4.4

-4.2 _{(LaFe}

13-xGax)

c

o

hesive Energy

(ev/atom)

Ga content (x)

0 1 2 3 4 5 6 -0.1

0.0 0.1 0.2 0.3 0.4 0.5 0.6 0.7 0.8

0.9 _{(LaFe}

13-xGax)

to

le

ra

n

c

e

Ga content (x)

8b 96i 4d 16k 16k(1) 16k(2)

0 1 2 3 4 5 6

-6.10 -6.05 -6.00 -5.95 -5.90 -5.85

(LaFe_{13-x}Mn_{x})

Co

he

s

iv

e E

ne

rgy

(

ev

/at

om

)

Mn content (x)

8b 96i 4d 16k 16k(1) 16k(2)

0 1 2 3 4 5 6

0.0 0.1 0.2 0.3 0.4 0.5 0.6 0.7 0.8

(LaFe_{13-x}Mn_{x})

tol

erance

Mn content (x)

0 1 2 3 4 5 6 -5.9

-5.8 -5.7 -5.6 -5.5 -5.4 -5.3 -5.2

(LaFe_{13-x}Ni_{x})

Cohesie

v

e

Energy(ev/at

om)

Ni content (x)

8b 96i 4d 16k 16k(1) 16k(2)

0 1 2 3 4 5 6

0.0 0.1 0.2 0.3 0.4 0.5 0.6 0.7 0.8

(LaFe_{13-x}Ni_{x})

to

ler

ance

Ni content (x)

8b 96i 4d 16k 16k(1) 16k(2)

**Figure 1. The cohesive energy and tolerance variation with the third element content x in LaFe****13-x****T****x ****(T = Cr, Cu, Ga, Mn, Ni) **

**with different space group Fm-3c and I4/mcm. **

**3.2. Fe-Fe Bond Length Change of LaFe****13-x****T****x**** (T **

**= Si, Al) **

tance and the number of nearest neighbors. Here, we will theoretically study the effects of Fe-Fe bond length change on the magnetic properties of NaZn13-type inter-metallic compounds.

In the cubic NaZn13 structure (space group Fm-3c), the rare earth atoms occupy the single 8a sodium site, while the Fe atoms are distributed over the two zinc sites, Fe1 (8b) and Fe2 (96i). The Fe1 atoms are surrounded by an icosahedron of 12 Fe2 atoms and possess a local symme-try peculiar to an FCC-like lattice. In the tetragonal structure (space group I4/mcm) the Fe atoms occupy four different sites. The Fe1 atoms (the 4d site) in icosahedron centers are surrounded by 12 Fe atoms in the sites Fe2(16k), Fe3(16l1) and Fe4(16l2). Previous investigations [10] have shown that the magnetic properties of the R-Fe-based compounds are determined predominantly by the Fe-Fe interaction, which is sensitive to the Fe-Fe dis-

In the experiments, LaFe13-*x*Al*x* crystallizes the cubic

NaZn13-type structure with the space group Fm-3c in the
range 1.04 ≤ x ≤ 7.15, and LaFe13-*x*Si*x* compounds are of

a single phase with the space group Fm-3c in the range
1.4 ≤ x ≤ 2.6 [11]. According to our previous works, Si
entering into the 96i site could stabilize the cubic
struc-ture of LaFe13-*x*Si*x* with x < 3.25, and for 3.25 < x < 5.25

**Table2. The crystallographic parameters a and c of LaFe****13-x****T****x ****(Al, Si) in Å, obtained from experiments (exp.) and **

**calcula-tions (cal.), and Ref. is the source of the experimental data. **

x a(cal) c(cal) a(exp) c(exp) Ref.

LaFe13-*x*Si*x* 2 11.470 11.463 [13]

3 8.035 11.485 7.994 11.363

4 7.997 11.501 7.974 11.542

5 7.967 11.595 7.954 11.720

LaFe13-*x*Al*x* 2 11.547 11.668 [14]

3 11.569 11.731

4 11.614 11.794

5 11.688 11.857

6 11.794 11.920

7 11.871 11.983

tive. **Table 2** shows the lattice parameters of LaFe13-xTx
(T = Si, Al) obtained from both the experiments [13] [14]
and calculations. The results correspond well to
experi-mental data. The bond lengths of Fe-Fe which play an
important role in magnetic properties can be evaluated.
In this subsection, the dependence of Curie temperature
on the Si/Al concentration is analyzed qualitatively.

In the experiment, the value of TC for the LaFe11.5Si1.5 compound is 188 K. Just as Givord et al. have pointed out, there are two types of exchange interactions, positive and negative, which depend on the length of Fe-dumb-bells. All the exchange interactions could be positive except the case associated with 96i-96i, 96i-8b, since the distances between these iron atoms are small.

In order to study the trend of Curie temperature
varia-tion, the distance between special sites and the related
exchange interaction should be investigated.** Figure 2 **

presents the bond lengths in LaFe13-*x*Si*x*, indicating that

the lengths of 96i-96i are shorter than 2.46 Å which can be considered as the threshold of switching exchange interaction. The distances between 96i-96i and 96i-8b decrease with increasing Si content, which are similar to that in the experimental trend. Notice that the bond lengths of 96i-8b are larger than 2.46 Å, then the varia-tion of exchange interacvaria-tion from 96i-8b pairs can be neglected. As far as iron pairs except 96i-96i are con-cerned, the positive exchange interactions associated with large bond lengths are weak, even though the intro-duction of Si atom has the effect of reintro-duction on them. Then the contribution to the exchange interaction from these iron pairs can also be neglected. In the next step, we will focus on the effect of 96i-96i lengths based on the variation of Curie temperature.

In the above subsection, the analysis of site preference behavior shows that Si atoms have a pronounced prefer-ence for occupying 96i site. On the one hand, the number of 96i-96i (Fe-Fe) dumbbell pairs reduces and the nega-tive exchange interaction with the increase of Si atom,

and in thus beneficial in improving the Curie temperature. on the other hand, bond lengths of 96i-96i pairs decrease with increasing Si content, and thus enhance the negative exchange interaction and lead to a lower Curie tempera-ture. So there is a competing mechanism arising from Si content increase, i.e. the variation of Curie temperature is not monotonic with the increment of Si concentration.

Givord *et al. [15] have shown that the threshold of *
switching Fe-Fe exchange interaction is 2.45 Å. In other
words, if the distance of Fe-Fe is shorter than 2.45 Å,
then the exchange interaction would be negative, if it is
larger than 2.45 Å, then it would be positive. In the
pre-sent calculation, the threshold of Fe-Fe exchange
interac-tion is taken as 2.46 Å, instead of 2.45 Å from the
ex-perimental analysis. This difference may be caused by a

systemic error in derivation of these quasi-

in-teratomic potentials.

*ab*

*initio*

**4. Conclusions and Discussions **

Pair potentials based on calculations and on

the lattice-inversion method have been used to calculate
the structural properties of a series of LaFe13-*x*T*x* (T = Cr,

Cu, Ga, Mn, Ni).The results show that Cr and Mn make
the cohesive energy decrease markedly, indicating that
these atoms can stabilize LaFe13-*x*T*x* with the cubic

NaZn13-type or its derivative tetragonal structure.

*ab*

*initio*

Furthermore, the increase of the Curie temperature of
LaFe13-*x*T*x* (T = Si, Al) with increasing Si concentration

can be qualitatively explained in terms of the distance dependence of the exchange interaction. The presented results indicate that simple pair potentials are useful for studying the structural properties of these kinds of inter-metallics.

**5. Acknowledgements **

0.0 0.5 1.0 1.5 2.0 2.5 3.0 3.5 2.42

2.44 2.46 2.48 2.50 2.52 2.54

Fe

-F

e dis

tance

Al/Si concentration (x)

96i-96i of LaFe_{13-x}Al_{x}
8b-96i of LaFe

13-xAlx

96i-96i of LaFe

13-xSix

8b-96i of LaFe

13-xSix

**Figure 2. Bond lengths (Å) of Fe-Fe pairs with the ternary element (Al/Si) content in LaFe13-xTx (T = Al, Si). **

2006CB605101. This work was also supported by the Young Natural Science Foundation of Jiangxi Blue Sky University.

**REFERENCES **

[1] S. G. Kim and K. Fukamichi, “Magnetic Properties of
La(Co1-*xCrx)*13 Compounds with an NaZn13-Type
Struc-ture,” *Journal of Alloys and Compounds*, Vol. 244, No.
1-2, 1996, pp. 146-150.

doi:10.1016/S0925-8388(96)02504-2

[2] S. Fujieda, A. Fujita and K. Fukamichi, “Large
Magneto-caloric Effect in La(FexSi1-*x)13 Itinerant-Electron *
Metamagnetic Compounds,” *Applied Physics Letters*, Vol.
81, No. 7, 2002, pp. 1276-12778.

doi:org/10.1063/1.1498148

[3] S. Fujieda, A. Fujita, K. Fukamichi, Y. Yamazaki and Y. lijima, “Giant Isotropic Magnetostriction of Itinerant- Electron Metamagnetic La(Fe0.88Si0.12)13Hy Compounds,”

*Applied Physics Letters*, Vol. 79, No. 5, 2001, pp.
653-655.doi:10.1063/1.1388157

[4] Ph. Oleinek, W. Kockelmann, K.-H. Muller, M.
Loewen-haupt and L. Schultz, “Neutron and X-ray Powder
Dif-fraction Study on the Compound NdFe10.75V1.25Ny,” *Jour- *

*nal of Alloys and Compounds*, Vol. 281, No. 2, 1998, pp.
306-311.doi:10.1016/S0925-8388(98)00782-8

[5] A. Fujita, S. Fujieda, Y. Hasegawa and K. Fukamichi,
“Itinerant-Electron Metamagnetic Transition and Large
Magnetocaloric Effects in La.FexSi1Àx.13 Compounds and
Their Hydrides,” *Physical Review B*, Vol. 67, No. 10,
2003, pp. 104416-104428.

doi:10.1103/PhysRevB.67.104416

[6] X. B. Liu, Z. Altounian and A. D. Beath, “Structure and
magnetic properties of La.Fe0.88Al0.12)13Cx interstitial
compounds,” *Journal of Applied Physics*, Vol. 95, No. 11,

2004.

[7] Y. F. Chen, F. Wang and B. G. Shen, *et al.*, “Magnetic
Properties and Magnetic Entropy Change of LaFe11*.*5
-Si1*.*5H*y *Interstitial Compounds,” *Journal of Physics*:* *
*Con-densed Matter*, Vol. 15,No. 7, 2003, pp. L161- L167.
doi:10.1088/0953-8984/15/7/102

[8] O. Moze, W. Kockelmann, J. P. Liu, F. R. de Boer and K.
H. J. Buschow, “Magnetic Structure of LaFe10.8Al2.2 and
LaFe10.8Al2.2N3 Cluster Compounds,” *Journal of Applied *

*Physics*, Vol. 87, No. 9, 2000, pp. 5284-5286.
doi:10.1063/1.373322

[9] Y. Liu, N. X. Chen and Y. M. Kang, “Virtual Lattice
Technique and the Interatomic Potebtials of Zinc-blend-
type Compounds,” *Moderen Physics Letters B*, Vol. 16,
No. 5-6, 2002, pp. 187-194.

doi:10.1142/S0217984902003622

[10] G. J. Wang, F. X. Hu, F. Wang and B. G. Shen, “Effects
of Fe-Fe Bond Length Change in NaZn13-Type
Intermet-allic Compounds on Magnetic Properties and Magnetic
Entropy Change,” *Chinese Physics*, Vol. 13, No 4, 2004.
[11] G. H. Rao, “Magnetism in R-T Intermetallic Compounds

with NaZn13-Type or its Derivative Structure,” *Journal of *

*Magnetism and Magnetic Materials*, Vol. 139, No. 1-2,
1995, pp. 204-208.

doi:10.1016/0304-8853(94)00442-0

[12] G. J. Wang, F. Wang, N. L. Di, B. G. Shen and Z. H.
Cheng, “Hyperfine Interactions and Band Structures of
LaFe13-*xSix Intermetallic Compounds with Large *
Mag-netic Entropy Changes,” *Journal of Magnetism and Mag- *
*netic Materials*, Vol. 303, No. 1, 2006, pp. 84-91.
doi:10.1016/j.jmmm.2005.10.231

[14] H. Chang, N. X. Chen, J. K. Liang and G. H. Rao, “The-
oretical Study of Phase Forming of NaZn13-Type Rare-
Earth Intermetallics,” *Journal of Physics*:* Conden- sed *
*Matter*, Vol. 15, No. 2, 2003, pp. 109-120.

doi:10.1088/0953-8984/15/2/311

[15] Y. F. Chen, F. Wang, B. G. Shen, F. X. Hu, J. R. Sun, G.

J. Wang and Z. H. Cheng, “Magnetic Properties and
Magnetic Entropy Change of LaFe11*.*5Si1*.*5Hy Interstitial
Compounds,” *Journal of Physics*:* Condensed Matter*, Vol.
15, No. 7, 2003, pp. L161-L167.